Delft University of Technology
The nephelauxetic effect on the electron binding energy in the 4fq ground state of lanthanides in compounds Dorenbos, Pieter DOI 10.1016/j.jlumin.2019.116536 Publication date 2019 Document Version
Accepted author manuscript Published in
Journal of Luminescence
Dorenbos, P. (2019). The nephelauxetic effect on the electron binding energy in the 4fq ground state of lanthanides in compounds. Journal of Luminescence, 214, .
https://doi.org/10.1016/j.jlumin.2019.116536 Important note
To cite this publication, please use the final published version (if applicable). Please check the document version above.
Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy
Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.
The nephelauxetic effect on the electron binding energy in the 4fq
ground state of lanthanides in compounds.
Delft University of Technology, Faculty of Applied Sciences,
Department of Radiation Science and Technology, Section Luminescence Materials,
Mekelweg 15, 2629 JB Delft, Netherlands email:email@example.com
tel: +31 15 2781336
(Dated: July 10, 2019)
In the construction of a vacuum referred binding energy (VRBE) diagram with the lanthanide 4fq ground states, always a compound independent variation with the number q = 1 to 14 is assumed. Experimental data from thermo-luminescence, intervalence charge transfer bands, and thermo-bleaching studies provide first indications that a minor compound dependence does exist. To explain its origin we will first apply the Jørgensen spin pairing theory to reproduce the VRBE in the ground states of the free di- and trivalent lanthanide ions which is equivalent to the 3rdand 4th ionization potentials of the lanthanide atoms. By combining experimental data and calculated trends therein, the relevant Racah E1, Racah E3, and spin orbit coupling ζff parameters for all di-,
tri-, and tetravalent free ion lanthanides are derived. Using that as input for the spin pairing theory, the characteristic zigzag shapes in VRBE as function of q, as derived from ionization potentials, are nicely reproduced. Because of the nephelauxetic effect the parameter values are lowered when lanthanides are in compounds. How that reduction affects the VRBE curves will be treated in this work.
The energy needed for an electronic transition from a lanthanide impurity state to a host valence band (VB) or conduction band (CB) state or vice versa provides information on the location of that impurity state within the band gap of the compound . Hole release from a lanthanide to the VB or electron release to the CB can be probed by thermoluminescence (TL) or by photoconductivity (PC) techniques. Electron transfer from the VB-top to a lanthanide or from a lanthanide to the CB-bottom are manifest as so-called charge transfer (CT) or intervalence charge transfer (IVCT) bands in absorption or luminescence excitation spectra.
From gathering information on CT-energies always the same characteristic variation in lanthanide ground state level location with the number of electrons in the 4f-orbital appears. This has led to empirical models to construct so-called host referred binding energy (HRBE) schemes with all divalent and all trivalent lanthanide 4fn ground state locations with respect
to the host bands. In 2012 the chemical shift model was developed  to convert such HRBE scheme into a vacuum referred binding energy scheme (VRBE) where all energies are referred to the vacuum level, i.e., the energy of an electron with zero kinetic energy in the vacuum.
Figure 1 shows the VRBE scheme for YPO4. The zigzag curve Ln2+/3+ connects the 4fq
ground state locations of divalent lanthanides. The energy difference with the CB-bottom is then the energy needed for electron ionization from Ln2+ that can be probed with TL or PC,
see for example arrow 1 for Nd2+. The same curve represents the electron acceptor levels of
the trivalent lanthanides. The energy difference with the CB-bottom is then the trivalent lanthanide electron trapping depth (see arrow 2 for Tm3+). The energy difference with
the VB-top is equivalent to the CT-band energy observed in excitation spectra of trivalent lanthanide luminescence (see arrow 3 for Yb3+). The zigzag curve Ln3+/4+ connects the
ground state locations of the trivalent lanthanides but can equally well be treated as the curve that connects the CB electron acceptor states of the tetravalent lanthanides. The energy difference with the VB-top is the energy needed for hole ionization from Ln4+ that
can be probed with TL (see arrow 4 for Pr4+ and arrow 5 for Tb4+).
During the past two decades, the shapes of the two zigzag curves were revised several times to eventually evolve in the latest ones from  that was used for Fig. 1. Since there
were no experimental indications for a compound dependence, the same zigzag shapes are used for all type of compounds. However recently, indications that the trivalent lanthanide zigzag curve must be compound dependent were found . With TL, the energy for hole release from Pr4+ was compared with that from Tb4+ for various compounds. Without such dependence, one expects that the energy difference will be constant. However that difference changes by about 0.1 to 0.15 eV when going from a phosphate, to silicate, to aluminate compound.
By comparing TL-data on electron release from divalent lanthanides with 60 years old thermo-bleaching data, one can also derive evidence for a compound dependence in the Ln2+/3+ binding energy curve. Figure 2 shows the thermoluminescence glow curves due to
the release of an electron trapped on divalent Er, Nd, Ho, Dy, and Tm in GdAlO3 which
then recombines with a hole trapped on Ce3+to generate Ce3+ 5d-4f luminescence . Glow peak analysis shows that a 0.01 eV increase in trapping depth already leads to ≈3K shift of the glow peak maximum Tm which demonstrates a very high sensitivity of Tm to the precise
shape of the Ln2+/3+ VRBE curve. The maximum temperature of the glow peak for Nd from the left hand side of the VRBE curve falls in between that of Er and Ho from the right hand side. The same applies to other oxides like YPO4 and LaPO4 . This is consistent
with the Ln2+/3+ VRBE curve in Fig. 1 as illustrated by the horizontal dashed line.
Fig. 3 shows results on the thermobleaching of divalent lanthanide absorption bands in CaF2:Sm2+;Ln3+ (Ln = Er, Ho, Nd, Dy) reproduced from the 1969 work of Arkangelskaya
et al. . Prior to the bleaching, electrons are transferred from Sm2+ to the trivalent
lanthanide by photon excitation. It creates absorption bands of divalent Er, Ho, Nd, or Dy. Next, the crystal is heated while monitoring the absorption intensity. The moment electrons can escape from the divalent lanthanide ground state, a bleaching of the absorption band is observed and one can define the temperature T50 where absorption has bleached by 50%.
T50 for Er, Ho, and Dy in CaF2 appears at about 290 K higher temperature then the Tm for
the same lanthanides in GdAlO3. This means that the electron trap for all three lanthanides
in CaF2 is a fixed amount deeper as compared to GdAlO3. Such fixed amount is consistent
with a compound independent shape of the VRBE curve. Note that the T50 for Nd falls
in between that of Ho and Dy in CaF2 whereas the glow peak of Nd in GdAlO3 falls in
between that of Er and Ho. This is not consistent with a compound independent shape. It suggests that in CaF2 the Dy, Ho, and Er divalent ground states are raised by about 0.15 eV
with respect to that of Nd2+. Considering above findings, we need to introduce a compound
dependence in the shape of the zigzag curves that should be of the order of few 0.1 eV. In this work we will demonstrate that by combining the nephelauxetic effect on the 2s+1L
level energies with the spin pairing theory of Jørgensen [6, 7] this can all be explained. The typical zigzag shapes in the binding energies for the 2+ and 3+ lanthanide ions also appear in the 3rd and 4th ionization potentials of the lanthanides, and it was long
time ago qualitatively explained with the spin pairing theory of Jørgensen [6, 7]. In that theory the interelectron Coulomb repulsion between the 4f electrons in the free lanthanides is parameterized by the Slater-Condon Fk (k = 0, 2, 4, 6) parameters and the spin-orbit coupling parameter ζff. In this work we will apply the spin pairing theory to quantitatively
reproduce the ionization potentials where we will follow a somewhat different route than in previous attempts.
The parameters of interelectron repulsion that determine the binding energy in the ground state multiplets equally well determine the binding in the excited state2S+1L
J multiplets of
the lanthanides. Figure 4 shows the energies of the 132S+1LJ 4f2energy levels for Pr3+as free
ion from , in LaF3 from [9, 10], and in La2O3 from  relative to that of the 3H4 ground
state. In compounds, the excited state energies are lowered with respect to the ground state due to a decrease in interelectron repulsion which is attributed to the nephelauxetic effect. Nephelauxetic is Greece for cloud expansion. It has been studied in great detail in many papers to explain the excited state energies of the lanthanides in compounds, but its effect on the VRBE of the lanthanide ground states has never been studied. One expects that changes in the interelectron repulsion will affect the ground state energies with respect to the vacuum level which, unless the change is the same for each lanthanide, implies that the two zigzag curves in Fig. 1 should be compound dependent. The results in Fig. 2 and Fig. 3 suggest that when going from fluorides to oxides, the ground state energy of divalent Dy, Ho, and Er on the right hand branch lower by about 0.15 eV with respect to that of divalent Nd on the left hand branch. Similar applies for the ground state energy of Tb3+ from the
right hand branch with respect to that for Pr3+ from the left hand branch. In this work we will first establish the Slater Fk and ζ
ff parameters for the di, tri, and
tetravalent free lanthanides by combining experimental data with calculated trends on how they change with the number of 4f electrons. Next the contribution of the interelectron repulsion to the binding energy in the ground states is determined. By using the data on
the 3rd and 4th ionization potentials we will derive smoothly varying functions with q for
the binding of a 4f electron to the nucleus with the [Xe] core configuration. Finally the effect of the chemical shift, the lanthanide contraction and the nephelauxetic effect on the VRBE in the lanthanide ground state multiplets when in a chemical environment will be treated. We will show that the nephelauxetic effect can lower the VRBE for the right hand branch(q > 7) of the zigzag curve by about 0.5 eV depending on the type of chemical environment or inorganic compound. This nephelauxetic lowering explains the observation in Fig. 2 and 3. The amount of nephelauxetic variation within the oxide compounds remains within ±0.1 eV and this is consistent the hitherto used approximation that the shape of the VRBE curves is invariant within ±0.1 eV.
The theory on the energy differences between the 4fq levels within a lanthanide ion is
well-established. Always the 4fq ground state is then the level of reference, which is placed
conveniently at energy zero as in Fig. 4. In this work we are interested in the energy differences between the ground states of two different lanthanides, and then we need a common reference of energy like the vacuum level in Fig. 1. Knowledge on these energy differences provides us with the shapes of the zigzag curves in binding energies. The energy differences within the lanthanides must be strongly tied with the energy differences between the lanthanides. Once this is established theoretically, knowledge on energy differences within a lanthanide can be utilized to determine energy differences between lanthanides.
For a free lanthanide ion, each electron in the 4fq orbital has the same interaction with the nucleus and with the electrons of its closed shell [Xe] configuration . This means that the energy differences between the 4fq levels within a lanthanide are, ignoring spin-orbit
inter-action, only determined by the repulsive Coulomb interaction between the electrons within the 4fq orbitals. The levels are like in Fig. 4 usually labelled with the 2s+1L
J term symbols
where L, S, and J are the quantum numbers for angular momentum, spin momentum, and total momentum of all q electrons together. The Coulomb repulsion between 4fq electrons is commonly expressed by the Slater integrals, and the value of those integrals for each 4fn
LS-term can be expressed with the four Slater-Condon parameters F0, F2, F4, and F6. These are all positive numbers that we will express in eV, and are determined exclusively by
the radial functions R4f(r). Calculations on the free lanthanide ions by Ma et al.  reveal
that F4 ≈ 0.625F2and F6 ≈ 0.45F2. The proportionality constants are almost independent
on atomic number and valence (2+, 3+, 4+). An LS-term will be further split by the spin orbit coupling leading to 2J + 1 different 2s+1LJ levels.
Optical spectroscopy of a lanthanide as a free ion or as a dopant in a compound provides detailed information on the excited state level energies with respect to the ground state. To understand and reproduce the rich level structure of the lanthanides, interactions between 4f electrons and with the crystal field were parameterized in terms of the Fkparameters, the
spin orbit coupling parameter ζff, the two body configuration interaction or Trees parameters
α, β, and γ, the Bqk crystal field parameters, and additional parameters of less importance
. The parameter values can then be obtained by fitting the theoretical expressions to the experimentally observed 2s+1LJ level energies. The crystal field parameters depend on
the site symmetry and bond lengths. The Fk parameters appear not to correlate with
the crystal field parameters but to the nephelauxetic effect . Tanner and Yeung  reviewed the experimental parameters for Pr3+ as free ion and for Pr3+in compounds paying special attention to the nephelauxetic effect and how that relates to the reduction of the Fk
parameters. Their conclusion based on a careful analysis and following ideas of Morrison [16, 17] and Newman  is that the parameter reduction and nephelauxetic effect is tied to the polarizability of the surrounding ligands. Since the Fk and the spin orbit coupling
parameter ζff are the dominant parameters that determine level energies we will only consider
the effect of those parameters on the VRBE in the ground state 4fq level. The two body
interaction parameters that emanate from second order perturbation theory , the crystal field parameters and others will not be further considered.
Instead of the Fkparameters often the E0, E1, E2, and E3 Racah parameters are used to
parameterize the inter-electron repulsion. They are positive numbers (energies) and linear combinations of the Fk parameters as in the following expressions.
E0 = F0− 2 45F 2− 1 33F 4− 50 1287F 6 ≈ F0− 8.08 × 10−2 F2 (1) E1 = 14 405F 2 + 7 297F 4 + 350 11583F 6 ≈ 6.29 × 10−2 F2 (2) E2 = 1 2025F 2− 1 3267F 4 + 175 1656369F 6 ≈ 3.50 × 10−4 F2 (3)
E3 = 1 135F 2+ 2 1089F 4− 175 42471F 6 ≈ 6.70 × 10−3 F2 (4)
Using the more or less constant ratios between the Fk parameters as established in the
calculations by Ma et al.,  the E1 , E2, and E3 Racah parameters can be approximately
expressed in terms of F2. Note that E3 is about ten times smaller than E1. The energy dif-ferences between the2s+1L
J levels within the lanthanides are independent on F0. Therefore,
spectroscopy cannot supply an experimental value for the F0parameter and, as consequence, the E0 Racah parameter.
The same parameters that control the separation between the 4fq levels within a
lan-thanide ion also control the binding energy in the ground state with respect to the vacuum level. We will use the expression from  for the total energy E(4fq, Q, vacuum) (in short
E(4fq) or E(4fq, Q)) of all q electrons in a 2s+1L
J 4fq-state E(4fq) = −qW −q(q − 1) 2 (E ∗− E0) + 9 13[ q(q − 1) 2 + n(S)]E 1+ m(L)E3+ p(S, L, J )ζ ff (5) E(4fq, Q) = c(q, Q) + s(q, Q) (6)
Here −W represents the binding energy of one 4f electron to the nucleus together with the [Xe] electron core. E∗ is a parameter to account for the stabilization of 4f electrons due to the increase of the effective nuclear charge from one lanthanide to the next. The first two terms together are assumed to be a smooth, but yet unknown, function with q. It will be denoted as function c(q, Q). The last three terms together define s(q, Q) and contain the e-e repulsion and spin orbit interaction in a 2s+1LJ state of the 4fq configuration. We added the
variable Q to the functions E, c and s in Eq. (6) to denote the valence (Q = 2+, 3+, or 4+) of the lanthanide. n(S), m(L), and p(S, L, J ) are coefficients that emanate from Jørgensons spin pairing theory. Column 6, 8, and 9 of Table I lists the values for those coefficients for the 2s+1L
J ground state term symbols in column 5. Columns 7 shows the coefficients for the
E1 contribution to Eq. (5).
The energy E4f(q, Q, A) needed to remove an electron from the ground state of the 4fq
configuration of an LnQ in a chemical environment A, and to bring it to the vacuum level is
TABLE I: The coefficients for the energy terms of the interelectron repulsion and spin-orbit inter-action for lanthanides with the 4fq configuration in the refined spin pairing energy theory.
q Ln2+ Ln3+ Ln4+ g.s. n(S) 139[q(q−1)2 + n(S)] m(L) p(S, L, J ) 0 – La Ce 1S0 0 0 0 0 1 La Ce Pr 2F 5/2 0 0 0 -2 2 Ce Pr Nd 3H4 -1 0 -9 -3 3 Pr Nd Pm 4I 9/2 -3 0 -21 -7/2 4 Nd Pm Sm 5I4 -6 0 -21 -7/2 5 Pm Sm Eu 6H 5/2 -10 0 -9 -3 6 Sm Eu Gd 7F0 -15 0 0 -2 7 Eu Gd Tb 8S 7/2 -21 0 0 0 8 Gd Tb Dy 7F6 -15 9 0 -3/2 9 Tb Dy Ho 6H15/2 -10 18 -9 -5/2 10 Dy Ho Er 5I8 -6 27 -21 -3 11 Ho Er Tm 4I15/2 -3 36 -21 -3 12 Er Tm Yb 3H4 -1 45 -9 -5/2 13 Tm Yb Lu 2F7/2 0 54 0 -3/2 14 Yb Lu – 1S0 0 63 0 0 E4f(q, Q, A) = E(4fq, Q, A) − E(4fq−1, Q + 1, A) (7)
In early treatments on this energy difference for the free lanthanides, the Racah and ζff
parameters were assumed independent on q and Q [7, 21]. Van der Sluis and Nugent  realized that one should take a q dependence into account. However, in Eq. (7) there is also a Q and A dependence which, different from previous work, will be taking into account here. Apart from La2+ and Gd2+, E
4f(q, 2+, vacuum) and E4f(q, 3+, vacuum) are equivalent
to the negative of the 3rd and 4th ionization potentials of the lanthanide atoms. For La2+
and Gd2+ the lowest 4fq−1 5d level is the ground state and the ionization energy must then
be corrected for the 4fq to 4fq−15d energy difference. The E
4f(q, Q, vacuum) values as also
compiled in  are reproduced in Table II.
TABLE II: Atomic number Z, E4f(q, Q, vacuum) (in eV) and the Shannon ionic radii R(q, Q) in
pm of the divalent and trivalent lanthanide ions. We used the tabulated radii for lanthanides in 8-fold coordination from .
Z Ln E4f(q, 2+) E4f(q, 3+) R(q, 2+) R(q, 3+) 57 La -18.286 – 148.7 130.0 58 Ce -20.198 -36.758 147.0 128.3 59 Pr -21.624 -38.98 145.3 126.6 60 Nd -22.102 -40.6 143.7 125.0 61 Pm -22.369 -41.2 142.2 123.4 62 Sm -23.601 -41.6 140.7 121.9 63 Eu -24.92 -42.97 139.3 120.5 64 Gd -20.335 -44.5 137.9 119.2 65 Tb -21.91 -39.37 136.6 117.9 66 Dy -22.89 -41.2 135.4 116.7 67 Ho -22.84 -42.4 134.3 115.6 68 Er -22.74 -42.5 133.2 114.5 69 Tm -23.68 -42.4 132.2 113.5 70 Yb -25.03 -43.56 131.3 112.5 71 Lu – -45.25 – 111.7
c(q, Q, ) − c(q − 1, Q + 1) between two expected smooth functions is again expected to be a smooth function. The difference S(q, Q) ≡ s(q, Q) − s(q − 1, Q + 1) can be computed by using experimental and or best estimated values for the Racah parameters and ζff and the
coefficients from Table I. By subtracting the S(q, Q) parts from the listed E4f(q, Q, vacuum)
values in Table II, we will first derive the smooth functions C(q, Q). For divalent and triva-lent free lanthanides they will indeed turn out to be smoothly varying with q. Next we will use experimental or estimated values for the Racah parameters in compounds like LaF3,
LaCl3, YPO4, and La2O3 to explore how that affects the shape of the zigzag curves in
III. RESULTS ON THE LANTHANIDES IN VACUUM
To employ Eq. (7) to reproduce the binding energy curve for the divalent and trivalent lanthanides we need the Slater parameters (or Racah parameters) and ζff, for the divalent,
trivalent and tetravalent lanthanides. For that we will make use of the calculated parameters by Ma et al. . To very good approximation the Fk and ζ1/4
ff increase linearly with the
atomic number Z, or equivalently with the number of electrons in the 4f-orbital. Therefore, instead of compiling the values for each lanthanide individually we can work with the linear relationships that are reproduced in Table III.
TABLE III: The linear relationships with atomic number Z for the calculated Slater parameters and calculated ζff1/4 for divalent, trivalent, and tetravalent free lanthanide ions. Data are from  and in eV.
F2 F4 F6 ζff1/4
Ln2+ −16.17 + 0.456Z −10.24 + 0.286Z −7.400 + 0.206Z 2.42510−5(Z − 32.73)
Ln3+ −11.63 + 0.403Z −7.233 + 0.251Z −5.187 + 0.181Z 2.26610−5(Z − 29.73) Ln4+ −8.981 + 0.377Z −5.448 + 0.234Z −3.866 + 0.168Z 2.18310−5(Z − 27.64)
Figures 5, 6, 7 show the experimentally known values for the Slater parameters for the free di-, tri-, and tetravalent lanthanides. That of the divalent lanthanides Ce, Eu, and Er are from [24–26], the trivalent lanthanides Pr, Nd, Er, Tm from [14, 27–29], and the tetravalent Nd, and Yb from [27, 30]. The dashed lines are the calculated linear relationships from Table III corrected with a constant value chosen such that the lines run through the experimental data points. The values of the constants are written within brackets along the dashed lines. Although only a limited set of experimental data is available, it appears that the calculated increase of Fk with atomic number is very well confirmed by the data. The needed constant
energy shift appears not to depend much on the lanthanide charge. Note that the value for all three Fk parameters increase with the charge Q of the lanthanide but that the rate of
change with Z decreases with Q.
Figure 8 shows experimental data on the spin-orbit coupling parameters ζff for the free
lanthanides. Ce2+ is from , Pr3+, Nd3+, and Nd4+ from , Eu2+ from , Er2+ from
, Er3+ from , Tm3+ from , and Yb4+ from . The solid curves connect the calculated results from  that are listed in Table III. The curves are shifted with a small
amount to adjust them better to the experimental data.
In the following we regard the dashed lines and curves in Figure 5, 6, 7, and 8 as our best representatives for the free ion Fk and ζ
ff values. It provides with Eq. (2) and Eq. (4)
all the parameters needed to calculate with Eq. (5), Eq. (7) and Table I the spin pairing contributions S(q, Q) to the binding energies E4f(q, Q, vacuum).
IV. RESULTS ON THE LANTHANIDES IN A CHEMICAL ENVIRONMENT
When lanthanides are placed in a chemical environment one has to deal with the interac-tions between the 4f electrons with that chemical environment. The main interaction is the Coulomb repulsion with the surrounding negative charge from the anions. This repulsion generates a chemical shift in binding energy towards less negative values. The nature, the size, and compound variation therein can be treated with the chemical shift model intro-duced in 2012 . Effectively a 2+ lanthanide is surrounded by 2- charge at a screening distance R2+. The screening distance appears slightly larger than the Shannon ionic radius
R(q, 2+) of the lanthanide in Table II. Similarly a 3+ lanthanide is screened by 3- charge at screening distance R3+ that is somewhat smaller than R2+. As a consequence the chemical
shift for Ln3+ will be slightly more than a factor 3/2 larger than for Ln2+. The U (6, A)-value for Eu defined in Eq. (8) is then reduced from the free Eu ion value of 18.05 eV to values that appear to range between 7.6 eV and 6.1 eV for Eu in inorganic compounds . It is for example 7.09 eV for YPO4 in Fig. 1 as indicated by the dashed arrow.
U (6, A) = E4f(7, 2+, A) − E4f(6, 3+, A). (8)
The changing U (6, A) value is directly linked to a compound dependent screening dis-tance. For compounds with strongly bonded anion ligands as in fluorides, the ligands cannot optimally screen the lanthanide charge which, within the chemical shift model, translates to a larger screening distance, relatively small chemical shift and large U (6, A). When ligands are more weakly bonded as in chlorides, bromides, iodides screening is more efficient lead-ing to smaller screenlead-ing distances, larger chemical shift, and smaller U (6, A). For the pure lanthanide metals screening is most efficient and chemical shift is maximal and U (6, A) be-comes minimal. The empirical relation between U (6, A) and the chemical shift E(7, 2+, A) or E(Eu, 2+, A) for divalent Eu is given by Eq. (9) and Eq. (10) from .
E(Eu, 2+, A) = 18.05 − U (6, A)
0.777 − 0.0353U (6, A) (9)
E(Eu, 3 + A) = E(Eu, 2+, A) + 18.05 − U (6, A) (10) Above equations all apply to Eu. Because of the lanthanide contraction, the screening radius RQ will decrease and the size of the chemical shift will increase from the beginning
towards the end of the lanthanide series. Assuming that the screening radius changes pro-portional with the difference in ionic radius of Eu this results, next to an upward shifting, also into a tilting of the free ion binding energy curve. One may write
E4f(q, Q, A) = E4f(q, Q, vacuum) + E(Eu, Q, A) + α(Q)(R(Eu, Q) − R(q, Q)) (11)
where a tilt parameter of α(3+) = 0.11 eV/pm and α(2+) = 0.075 eV/pm provided best agreement with experimental derived binding energy curves in .
In the construction of the VRBE diagrams for the lanthanides in compounds, the only compound dependent parameter is the U (6, A) value. A compound dependent tilt was always ignored, and possible effects of compound dependence of Racah values were also never addressed. Figure 9 shows the Fk parameters for the trivalent lanthanides in LaCl
as reported by Yeung and Tanner . The same figure shows the linearized parameters for the free ions reproduced from Figure 6. The parameters for LaCl3 are about 5% smaller
than that for the free ions which must be attributed to the nephelauxetic effect.
The dependence of the Fk parameters on type of compound and the nephelauxetic effect
has been studied many times, but always with the aim to better understand the 4fn excited state level energies like in Fig. 4 with respect to the ground state. It was never aimed to describe the VRBE in the ground state. Tanner and Yeung  recently collected and analyzed the Fk values for Pr3+ in almost 40 different chemical environments. Parameters
selected for several representative compounds are compiled in Table IV. That for LaF3 are
TABLE IV: Fk parameters for Pr3+ in various chemical environments in units of eV. The ones for vacuum are from this work and the others from the compilation in .
A F2 F4 F6 ζf β(3+, A) U (6, A) vacuum 8.929 6.495 4.464 0.0948 1 18.05 LaF3 8.555 6.269 4.068 0.0927 0.958 7.51 LaCl3 8.486 6.228 4.088 0.0927 0.950 6.80 YPO4 8.410 6.158 4.026 0.0925 0.942 7.09 La2O3 8.254 6.141 4.039 0.0913 0.924 6.45 V. DISCUSSION
By combining experimentally determined values for the free lanthanide Fk and ζff
pa-rameters with trends that emanate from calculated values, a set of best estimates for the free divalent and free trivalent lanthanides were obtained in Figures 5, 6, 7, 8. With the spin pairing theory one can now compute the contribution S(q, Q) from the Racah E1, E3, and ζff parameters to the VRBE E4f(q, Q, vacuum) in the ground states of the lanthanides. The
obtained values for S(q, 2+) and S(q, 3+) are listed in Table V. The values S(q, 3+) for the trivalent lanthanides are connected by curve 1) in Fig. 10. The separate contributions from E1, E3, and ζ
ff to S(q, 3+) are shown as curves 2, 3, and 4.
The most important feature is the hump between q is 7 and 8. Column 7 of Table I shows that E1 does not contribute for q is 1 to 7 but for Tb3+ with q=8 there is a
9E1(8, 3+) ≈ 0.57F2(8, 3+) = 6.7 eV contribution to the e-e repulsion. The contribution
slowly decreases to 63E1(14, 3+) − 54E1(13, 4+) = 5.2 eV for Lu3+ as illustrated with curve 2). The spin-orbit contribution illustrated by curve 4) is first slowly increasing with q followed by a 0.71 eV downward jump between q is 7 and 8 and then again slowly increasing. The E3 contribution creates the oscillating VRBE in the left and in the right hand branch of S(q, 3+).
The known E4f(q, Q, vacuum) values in Table II are shown as curves 1) in Fig. 11 and
12. By subtracting the S(q, Q) values one obtains the functions C(q, Q). The values are compiled in Table V and illustrated by curves 2) in Fig. 11 and 12. They are indeed varying smoothly with q. As a test, the C(q, Q) functions were re-calculated by using 5% augmented and 5% reduced values for the free ion Fk parameters. It has only significant effect for q > 7
TABLE V: Compilation of the values for C(q, Q) and S(q, Q) as derived from the spin pairing theory and the free divalent and trivalent lanthanide zigzag curves. Energies are in eV, q is the number of electrons in the 4fq ground state of Ln2+ and n = q − 1 the same for Ln3+.
n Ln C(q, 2+) S(q, 2+) C(n, 3+) S(n, 3+) 0 La -18.170 -0.116 – – 1 Ce -19.723 -0.475 -36.591 -0.167 2 Pr -21.087 -0.537 -38.370 -0.610 3 Nd -22.325 0.223 -39.895 -0.705 4 Pm -23.331 0.962 -41.387 0.187 5 Sm -24.390 0.789 -42.627 1.072 6 Eu -25.249 0.329 -43.870 0.900 7 Gd -25.901 5.566 -44.852 0.402 8 Tb -26.535 4.625 -45.792 6.422 9 Dy -27.084 4.194 -46.712 5.487 10 Ho -27.809 4.969 -47.524 5.089 11 Er -28.569 5.829 -48.478 5.998 12 Tm -29.243 5.563 -49.375 6.955 13 Yb -29.913 4.883 -50.191 6.631 14 Lu – – -51.066 5.816
as illustrated by the two dashed curves above and below curves 2) in Fig. 11 and 12. Note that a discontinuity appears between q is 7 and 8, and unless such discontinuity is supposed to be, we conclude that the used Fk and ζ
ff values must be reliable and that the spin pairing
theory is consistent. Curves 3) in Figures 11 and 12 show the VRBE curves after applying the shift and tilt operation of Eq. (11) where for displaying purpose a convenient value of 4 eV for E(Eu, Q, A) was chosen. These curves already mimic quite well the shape of the zigzag curves that are found experimentally for the lanthanides in compounds as in Fig. 1. In this work we intend to add the effect of the nephelauxetic reduction of Racah and ζ parameters on the shape of the binding energy curves. Since F2 is the most important parameter for the Racah E1 and E3 values it is convenient to introduce the nephelauxetic
β(Q, A) ≡ F
F2(Q, vacuum) (12)
to express not only the reduction in F2 but also in F4, F6, and ζff. Furthermore we
assume that the reduction is independent on q. The VRBE in the lanthanide ground state in a chemical environment A is now written as
E4f(q, Q, A) = C(q, Q) + β(Q, A)S(q, Q) + E(Eu, Q, A) + α(Q)(R(Eu, Q) − R(q, Q)) (13)
which now contains two compound dependent parameters β(Q, A) and the chemical shift for EuQ. Note that here the interaction C(q, Q) with the nucleus and [Xe] core is assumed compound independent. If a slight compound dependence were present most likely it will scale with the lanthanide ionic radius and then its effect can be incorporated by a somewhat modified value for α(Q). The chemical shifts for EuQ are entirely defined by the U (6, A) parameter via Eq. (9) and (10). Values for β(3+, A) for some representative compounds are listed in Table IV and others can be derived from the compilation of Pr3+ Fk(3+, A) parameters in. β(3+, A) is highest with typical values of 0.96 for the fluoride family of compounds like LaF3 and lowers progressively when moving to chlorides, bromides, and
iodides. Within the oxides it will scale with the electronegativity of the cations that binds the oxygen ligands (P > B > Si > Al). The U (6.A) parameter varies in an opposite fashion which suggests that β(3+, A) and U (6, A) are also tightly linked.
The dashed curve 4) in Fig. 12 illustrates the effect of an 8% reduction in β(3+, A) on the VRBE for the lanthanide ground states which resembles the situation in La2O3 with
U (6, A)=6.44 eV. The effect for the left hand branch (q < 8) of the lanthanide series is barely significant. However, the entire right hand branch (q > 7) is lowered by 0.51 eV for Tb3+ and 0.46 eV for Lu3+. The same for the divalent lanthanides is demonstrated by the
dashed curve 4) in Fig. 11 where the right hand branch is lowered by about 0.4 eV. The VRBE curve for fluorides with β(3+, A) ≈ 0.96 and U (6, A) 7.4 - 7.6 eV will run in between curves 3) and 4). The curves for sulfide and selenide compounds with U (6, A) values down to 6.1 eV are then expected to run below that for La2O3.
To explain the nephelauxetic effect, Morrison  suggested that a 4f electron will polarize the ligand electrons leading to energy lowering. In fact it describes a correlated motion between the 4f electron and the ligand electrons. The same applies for the 5d electron
of the 4fq−15d configuration. In the case of Ce3+ this interaction together with covalence
between the 5d-orbital and the ligands was used to establish a relation between the so-called 5d centroid shift and the electronegativity of the cations in the compound in . High electronegative cations bind the anion ligands strongly leading to low polarizability and small nephelauxetic effect. The chemical shift is caused by the screening of the lanthanide charge Q and such screening is also related to ligand polarizability. Indeed an empirical relationship between the U (6, A) parameter of the chemical shift model and the centroid shift for Ce3+ was demonstrated in . Considering that ligand polarizability is the common important parameter one may also expect a relationship between β(Q, A) and U (6.A).
With β(3+, A) ranging from 0.96 for the least polarizable fluoride compounds to about 0.90 for the highly polarizable sulfides and selenides, the lowering of the right hand branch in Fig. 12 is predicted to amount 0.2 eV to 0.6 eV. This gives about 0.4 eV spread over the entire family of inorganic compounds due to the nephelauxetic effect. The changes in the left hand branch are quite insignificant. Electron transfer from a lanthanide to a host band is always accompanied with strong lattice relaxation which leads to typically 0.8 eV wide excitation or absorption bands in optical spectra. With such broad bands the accuracy of level location determination is usually limited to several 0.1 eV, and that is the main reason that a compound dependence of the VRBE curve was never noticed.
The different behavior of Nd from the left hand branch of the VRBE curve from that of Er, Ho, Dy from the right hand branch, as noticed in the TL results of Fig. 2 and the thermobleaching results in Fig. 3, is now explained with a nephelauxetic lowering of the right hand branch of the VRBE curve. This is illustrated in Fig. 13 where the VRBE in the Ln2+ ground states from the left hand branch (levels a) and right hand branch (levels c) as
used in Fig, 1 are displayed separately. That of Eu2+ is placed at zero energy. The Nd2+
ground state falls in between that of Er and Ho as observed with TL for oxide compounds like GdAlO3 in Fig. 2. In thermobleaching data for CaF2, but also for SrF2  and for
BaF2 , Nd appears in between Ho and Dy, a situation that can be obtained by raising
the right hand levels c) by 0.15 eV to give the levels b) in Fig. 13. This agrees with the situation shown in Fig. 11 where curve 3) represents the VRBE in a compound without a nephelauxetic reduction or β = 1. Curve 4) pertains to La2O3 with β=0.92, and the right
hand branch has lowered by 0.4 eV. Fluorides have typical values of β=0.96 and the right hand levels will raise with about 0.2 eV with respect to that of La2O3.
The nephelauxetic lowering also applies to the right hand branch of the Ln3+/4+ zigzag
curve. It explains why in the sequence phosphates, silicates, aluminates the VRBE in Tb3+
from the right hand branch with respect to that in Pr3+ from the left hand branch lowers by about 0.1-0.15 eV as concluded from TL-studies in . The cation electronegativity decreases from P, to Si, to Al resulting in decreased oxygen ligand bonding, increased ligand polarizability, and increasing nephelauxetic lowering of the right hand branch.
VI. SUMMARY AND CONCLUSIONS
. We have applied the spin pairing theory of Jørgensen to establish the contribution of 4f interelectron repulsion to the VRBE in the ground state 4fq 2S+1L
J multiplets of
the free divalent and free trivalent lanthanides. For that we first determined the values of the Slater-Condon Fk and the spin orbit coupling ζ
ff parameters by combining known
experimental data with trends from computation. Different from previous work, we have taken the dependence of these parameters on q and on the valence Q (2+, 3+, 4+) of the free lanthanide into account. The derived binding energy of the 4f electrons to the nucleus plus the electrons in the closed [Xe] shells appear to show an expected smooth variation with q. From this we conclude that the used Fk and ζ
ff values are correct and that the spin
pairing theory is consistent.
The effect of reduction of the Fk and related E1 and E3 Racah parameters due to the
nephelauxetic effect on the binding energy when lanthanides are in a chemical environment has been explored. As first order correction the entire right hand branch of the binding energy curve for q > 7 is lowered by 9∆E1 ≈ 0.566∆F2 which in practice amounts to
several 0.1 eV. This already explains why the VRBE of Nd2+ is in between those of Ho and
Dy in CaF2 whereas it is in between those of Er and Ho in oxides. It also explains why the
VRBE in the Tb3+ ground state lowers by 0.1 to 0.15 eV with respect to that of Pr3+ in
going from phosphate to silicate to aluminate compounds.
In this work, we ignored a possible compound dependence in the tilt parameter α(Q) and of the smooth function C(q, Q). Such dependence will affect the entire 4fq VRBE
curve whereas the nephelauxetic ratio will only affect the right hand branch of that curve. This work has shown that the TL and thermo-bleaching techniques are sensitive enough to compare the VRBE for lanthanides from the left hand branch with that from the right hand
branch with an accuracy of few 0.01 eV. Then with such techniques one may carefully study small changes in the VRBE curve and relate that to a changing nephelauxetic ratio and or tilt factor.
The author thanks dr. E.R. Radzhabov for sharing his results on thermo-bleaching data presented at the LUMDETR conference in Prague and for bringing reference  to his attention.
 P. Dorenbos, Opt. Materials 69 (2017) 8.  P. Dorenbos, Optical Materials 91 (2019) 333.  P. Dorenbos, Phys. Rev. B 85 (2012) 165107.
 Hongde Luo, Adrie J. J. Bos, Pieter Dorenbos, J. Phys. Chem. C 120 (2016) 5916.
 V.A. Arkhangelskaya, M.N. Kiseleva, V.M. Shraiber, Soviet Physics Solid State, USSR, 11 (1969) 714 (p.869 in Russian)
 C.K. Jørgensen, Mol. Phys. 5 (1962) 271.
 C.K. Jørgensen, Modern Aspects of ligand Field Theory, North-Holland Publishing Company, Amsterdam, (1971).
 D.A. Wensky, W.G. Moulton, J. of Chem. Phys. 53 (1970) 3957.
 H.H. Caspers, H.E. Rast, R.A. Buchanan, J. Chem. Phys. 43 (1965) 2124.  W.T. Carnall, P.R. Fields, R. Sarup, The J. of Chem. Phys. 51 (1969) 2587.  O.K. Moune, M.D. Faucher, C.K. Jayasankar, A.M. Lejus, J. Lumin. 85 (1999) 59.
 J.S. Griffith, The theory of Transition-metal Ions (Cambridge University Press, London, 1961.  C.-G. Ma, M.G. Brik, Q.-X. Li, Y. Tian, Journal of Alloys and Compounds 599 (2014) 93.  Peter A. Tanner, Yau Yuen Yeung, J. Phys. Chem. A 117 (2013) 1072.
 E. Antic-Fidancev, M. Lemaitre-Blaise, P. Caro, New J. Chem. 11 (1987) 467.  C. Morrison, D.R. Mason, C. Kikuchi, Phys. Lett. A24 (1967) 607.
 C.A. Morrison, J. Chem. Phys. 72 (1980) 1001.  D.J. Newman, J. Phys. chem. solids 34 (1973) 541.
 K. Rajnak, B.G. Wybourne, The J. of Chem. Phys. 41 (1964) 565.  I. Kawabe, Geochemical Journal, 26 (1992) 309.
 D.A. Johnson, J. Chem. Soc. (a) (1969) 1525.
 K.L. Vander Sluis, L.J. Nugent, Phys. Rev. A 6 (1972) 86.
 R.D. Shannon, Acta Crystallogr. Sect. A: Cryst. Phys., Diffr., Theor. Gen. Crystallogr. 32 (1976) 751.
 Jean-Francois Wyart, Patrick Palmeri, Physica Scripta. 58, (1998) 368.
 J.-F. Wyart, W.-U L. Tchang-Brillet, S.S. Churilov, A. N. Ryabtsev, Astronomy and astro-physics 483 (2008) 339.
 Jean-Franqois Wyart, Jean Blake, William P. Bidelman, Charles R. Cowley, Physica Scripta, 56 (1997) 446.
 Jean-Francois Wyart, Ali Meftah, Jocelyne Sinzelle, Wan-U Lydia Tchang-Brillet, Nissan Spector, Brian R Judd, J. Phys. B: At. Mol. Opt. Phys. 41 (2008) 085001.
 A Meftah, S Ait Mammar, J-F Wyart, W-U L Tchang-Brillet, N. Champion, C. Blaess, D Deghiche, O Lamrous, J. Phys. B: At. Mol. Opt. Phys. 49 (2016) 165002.
 A. Meftah, J.-F.Wyart, N. Champion, W.-U L. Tchang-Brillet, Eur. Phys. J. D, 445 (2007) 35.
 Ali Meftah, Jean-FrancoisWyart, Wan-U Lydia Tchang-Brillet, Christophe Blaess, Norbert Champion, Phys. Scr. 88 (2013) 045305.
 P. Dorenbos, J. Lumin. 135 (2013) 93.
 Y. Y. Yeung, P. A. Tanner, J. Phys. Chem. A 119 (2015) 6309.  P. Dorenbos, Phys. Rev. B 65 (2002) 235110.
 P. Dorenbos, J. Lumin. 136 (2013) 122.
FIG. 1: The vacuum referred binding energy scheme for the divalent and trivalent lanthanide ground state levels in YPO4. For Pr3+ also the VRBE in the excited state 2S+1LJ multiplets
are drawn. Numbered arrows indicate electron or hole transitions. The horizontal dashed line illustrates that the VRBE for Nd2+ is in between that for Ho2+ and Er2+.
FIG. 2: Thermoluminescence glow curves from GdAlO3:Ce3+;Ln3+ (Ln = Er, Nd, Ho, Dy, Tm
when monitoring the Ce3+ emission at a heating rate of 1K/s. Data are retrieved from 
3 0 0 4 0 0 5 0 0 6 0 0 0 . 0 0 . 2 0 . 4 0 . 6 0 . 8 1 . 0 4 ) 3 ) 2 ) n o rm a liz e d o p ti c a l d e n s it y t e m p e r a t u r e ( K ) E r H o N d D y C a F 2: S m 2 +, L n 3 + 1 )
FIG. 3: Thermobleaching curves of 1) Er2+, 2) Ho2+, 3) Nd2+, and 4) Dy2+ 4f-5d absorption bands in CaF2;Sm2+;Ln3+ (Ln = Er, Ho, Nd, Dy) monitored at a heating rate of 0.25K/s. Data
FIG. 4: 4f2 energy level energies for Pr3+ as free ion in LaF3 and in La2O3. The drawn 1S0 level
for La2O3 is not from experiment but tentatively placed.
FIG. 5: Experimental data on the Fk parameters for the divalent lanthanides together with the calculated values from . Calculated values were shifted with an amount as indicated in eV within brackets along the dashed lines.
FIG. 6: Experimental data on the Fk parameters for the trivalent lanthanides together with the calculated values from . Calculated values were shifted with an amount as indicated in eV within brackets along the dashed lines.
FIG. 7: Experimental data on the Fk parameters for the tetravalent lanthanides together with the calculated values from . Calculated values were shifted with an amount as indicated in eV within brackets along the dashed lines.
FIG. 8: Experimental data on the ζff spin orbit coupling parameter for the free lanthanides together
with the calculated values from . Curve 1) calculated values for free Ln4+down shifted by 0.007
eV, 2) for the free Ln3+ down shifted by 0.005 eV, 3) for the free Ln2+ down shifted by 0.005 eV. The diamond shape, uptriangle, and down triangle data symbols are the experimental values for tetra-, tri-, and divalent lanthanides.
FIG. 9: FkSlater parameters derived from experimental data for the trivalent lanthanides in LaCl3
from . The dashed lines are based on calculated values for the free lanthanide ions. Calculated values were shifted with an amount as indicated in eV within brackets along the dashed lines to agree best with experimental data.
FIG. 10: The contribution of inter 4f-electron Coulomb repulsion S(q, 3+) (curve 1) to the VRBE in the ground state of the free trivalent lanthanides as calculated with the spin pairing theory. 2), 3), and 4) are the separate contributions from E1, E3, and ζff to the repulsion.
FIG. 11: Curve 1) shows the VRBE E4f(q, 2+, vacuum) in the ground state of the divalent
lan-thanides. The smooth solid curve 2) is C(q, 2+) obtained by subtracting the calculated spin pairing theory part S(q, 2+) from curve 1). Curves 3) is obtained after applying a chemical shift of 4 eV and a tilt operation with α(2+)=0.075 eV/pm. Dashed curve 4) represents the effect of 8% reduced Racah and ζ parameter values on binding energy.
FIG. 12: Curve 1) shows the VRBE E4f(q, 3+, vacuum) in the ground state of the trivalent
lan-thanides. The smooth curve 2) is C(q, 3+) obtained by subtracting the spin pairing theory part S(q, 3+) from curve 1). Curve 3) is obtained after applying a chemical shift of 4 eV and a tilt operation with α(3+)=0.11 eV/pm. Dashed curve 4) represents the effect of 8% reduced Racah and ζ parameter values on binding energy.
FIG. 13: VRBE energies in the Ln2+ground state with respect to that of Eu2+. Levels a) pertain to lanthanides from the left hand branch of the divalent lanthanide zigzag curve. Levels b) represent the right hand branch lanthanides in fluorides like CaF2 and levels c) in oxides like GdAlO3.